Luminescent Hydrogel Based on Silver Nanocluster/Malic Acid and Its Composite Film for Highly Sensitive Detection of Fe3+

Metal nanoclusters (NCs) with excellent photoluminescence properties are an emerging functional material that have rich physical and chemical properties and broad application prospects. However, it is a challenging problem to construct such materials into complex ordered aggregates and cause aggregation-induced emission (AIE). In this article, we use the supramolecular self-assembly strategy to regulate a water-soluble, atomically precise Ag NCs (NH4)9[Ag9(C7H4SO2)9] (Ag9-NCs, [Ag9(mba)9], H2mba = 2-mercaptobenzoic acid) and L-malic acid (L–MA) to form a phosphorescent hydrogel with stable and bright luminescence, which is ascribed to AIE phenomenon. In this process, the AIE of Ag9-NCs could be attributed to the non-covalent interactions between L–MA and Ag9-NCs, which restrict the intramolecular vibration and rotation of ligands on the periphery of Ag9-NCs, thus inhibiting the ligand-related, non-radiative excited state relaxation and promoting radiation energy transfer. In addition, the fluorescent Ag9-NCs/L–MA xerogel was introduced into polymethylmethacrylate (PMMA) to form an excellently fluorescent film for sensing of Fe3+. Ag9-NCs/L–MA/PMMA film exhibits an excellent ability to recognize Fe3+ ion with high selectivity and a low detection limit of 0.3 μM. This research enriches self-assembly system for enhancing the AIE of metal NCs, and the prepared hybrid films will become good candidates for optical materials.

Recently, the aggregation-induced emission (AIE) strategy has been used to enhance the photoluminescence of metal NCs, thereby enhancing its application in fluorescent sensing, light-emitting diodes, and other optoelectronic devices [20][21][22]. At present, the commonly used methods for AIE are solvent and cation-induced aggregation. However, these two methods cannot obtain ordered aggregates, resulting in instability and poor uniformity of nanocluster aggregation [23][24][25][26]. Therefore, an effective strategy for manipulating the spatial arrangement of nanostructured units to form a specific structure: self-assembly, was introduced to solve this problem. By regulating the non-covalent forces between multiple molecules (van der Waals forces, hydrogen bonds, electrostatic interactions, and π-π stacking), metal NCs, and other molecules form ordered aggregates with specific functions, which further improves the photoluminescence performance of the metal NCs [27][28][29]. The Ag 9 -NCs in an aqueous solution is in a nonfluorescent state. In order to regulate the aggregation behavior and AIE of Ag 9 -NCs, though the non-covalent interaction force dominated by hydrogen bonds, L-MA with hydroxyl and carboxyl functional groups is selected as a hydrogen bond donors, and Ag 9 -NCs, with carboxylate on the periphery, act as hydrogen bond acceptors. Firstly, phase behavior study on Ag 9 -NCs/L-MA mixed system was performed. Based on our previous study [40,41], c Ag9-NCs was fixed at 8 mM, while c L-MA was changed. It can be seen that different phase behaviors of the samples were obtained (Figure 1a). Compared with the solution without fluorescence (0~0.1 M L-MA) and the sample in the two-phase with weaker fluorescence intensity (0.1~0.25 M L-MA), the hydrogel with higher luminous intensity (0.25~0.5 M L-MA) was selected as the main research object. Once the hydrogels formed, the UV absorption exhibits a broad peak from 200 to 550 nm ( Figure 1d) and the electrons of the benzene ring system and C=O undergo π-π* and n-π* transitions, resulting in ultraviolet absorption bands. Moreover, orange-red fluorescence at 628 nm was excited by blue light at 470 nm ( Figure 1d) and it can be observed that as c L-MA increases, the fluorescence intensity of the hydrogel first increases and then decreases (Figure 1e,f). This is attributed to the fact that when c Ag9-NCs = 8 mM and c L-MA = 0.3 M, Ag 9 -NCs and L-MA self-assemble to form highly ordered aggregates, and L-MA sufficiently limits the ligands of Ag 9 -NCs, while when c L-MA is too high or too low, the uniformity of the formed aggregates is poor, and the self-assembly strategy cannot be effectively implemented, which leads to the weakening of fluorescence intensity. Thus, 8 mM Ag 9 -NCs/0.3 M L-MA hydrogel, which has the highest fluorescence intensity was selected as the typical sample.
Then, the dynamic change of fluorescence intensity with the hydrogel formation was also studied. Once Ag 9 -NCs and L-MA mixed, under the drive of non-covalent interaction forces, the fluorescent intensity of 8 mM Ag 9 -NCs/0.3 M L-MA hydrogel increased immediately within 30 min, achieving AIE effect. After about 1 h, the selfassembly process is almost complete, the fluorescence intensity stabilized and no longer changed (Figure 1g,h). Moreover, the peak position of the fluorescence spectrum has a slight blue shift with time. It is speculated that Ag 9 -NCs, L-MA and water molecules gradually formed the hydrogel through the hydrogen bonds, the vibration of the peripheral ligand of Ag 9 -NCs is restricted, and ligand-to-metal charge transfer occurred, resulting in a blue shift of the peak position. Thus, the AIE phenomenon of Ag 9 -NCs/L-MA hydrogel can be attributed to the limited intramolecular vibration and rotation of the ligand of Ag 9 -NCs, which inhibits the ligand-related non-radiative excited state relaxation and promotes radiation energy transfer. Furthermore, the average of lifetime of Ag 9 -NCs solution is 3.277 ns, while the average of the lifetime of 8 mM Ag 9 -NCs/0.3 M L-MA hydrogel increased to 7.4383 µs (Figure 1i, Table S1), which is approximately 2270 times that of Ag 9 -NCs solution. Therefore, the large Stokes shift (158 nm) and microsecond lifetime (7.4383 µs) indicate that it is essentially phosphors. Besides, the quantum yield of 8 mM Ag 9 -NCs/0.3 M L-MA hydrogel, measured using the integrating sphere, is 11.20%, which is higher than that of aggregates formed by the assembly of Ag 9 -NCs with other substances [42]. Longer fluorescence lifetime and higher quantum yield of Ag 9 -NCs/L-MA hydrogels make it excellent candidates for luminescent sensing materials.  Table S1), which is approximately 2270 times that of Ag9-NCs solution. Therefore, the large Stokes shift (158 nm) and microsecond lifetime (7.4383 μs) indicate that it is essentially phosphors. Besides, the quantum yield of 8 mM Ag9-NCs/0.3 M L-MA hydrogel, measured using the integrating sphere, is 11.20%, which is higher than that of aggregates formed by the assembly of Ag9-NCs with other substances [42]. Longer fluorescence lifetime and higher quantum yield of Ag9-NCs/L-MA hydrogels make it excellent candidates for luminescent sensing materials.   Figure S2). The confocal laser scan microscopy (CLSM) image shows that the tubes structure is accompanied by strong fluorescent properties. Further observation by TEM shows that these hollow tubes are composed of a large number of smaller diameter fibers (10-20 nm) ( Figure S3). Moreover, it can be seen in SEM that a small amount of hollow tubes are entangled to form a spiral (Figure 2d). It is speculated that the appearance of AIE can be attributed to the appearance of ordered hollow tube structure. The detailed formation mechanism of the hollow-tube structure of Ag 9 -NCs/L-MA hydrogel can be shown in Scheme 1. copy (CLSM) image shows that the tubes structure is accompanied by strong fluorescent properties. Further observation by TEM shows that these hollow tubes are composed of a large number of smaller diameter fibers (10-20 nm) ( Figure S3). Moreover, it can be seen in SEM that a small amount of hollow tubes are entangled to form a spiral (Figure 2d). It is speculated that the appearance of AIE can be attributed to the appearance of ordered hollow tube structure. The detailed formation mechanism of the hollow-tube structure of Ag9-NCs/L-MA hydrogel can be shown in Scheme 1.

Structural Analysis of the Hydrogel
In order to further analyze the mechanism of supramolecular self-assembly, a series of characterizations were carried out. Thermogravimetric analyses (TGA) can be used to measure the thermal stability of the studied substances ( Figure 3a). The decomposition temperature of L-MA is about 145 °C and the decomposition temperature of the H2mba ligand of Ag9-NCs is about 200 °C. After assembly, the decomposition temperature of the H2mba ligand of Ag9-NCs for Ag9-NCs/L-MA xerogel is about 260 °C, indicating that the stability of Ag9-NCs is further improved by supramolecular self-assembly.
Fourier transform infrared (FT-IR) is an effective tool for analyzing the supramolecular forces (Figure 3b). The broad peak of Ag9-NCs/L-MA xerogel at 2500 cm −1 to 3200 cm −1 represents the stretching vibration of the hydroxyl group, which is stronger and wider than that of Ag9-NCs, indicating the formation of hydrogen bonds in the system. The peak at 1700 cm −1 representing the stretching vibration of the C=O in the carboxyl group becomes weaker than that of L-MA after the gel is formed, and slightly shifts to a lower wave number, which represents the formation of hydrogen bonds and confirms that L-MA participates in the construction of the hydrogel. The peak at 3540 cm −1 represents that the hydroxyl groups in L-MA undergo intermolecular association through hydrogen bonds to form L-MA dimers, which disappear after gelation, indicating that L-MA forms hydrogen bonds with the peripheral ligands of Ag9-NCs. The peaks at 1537 cm −1 and 1377 cm −1 belong to the antisymmetric and symmetric stretching vibration of

Structural Analysis of the Hydrogel
In order to further analyze the mechanism of supramolecular self-assembly, a series of characterizations were carried out. Thermogravimetric analyses (TGA) can be used to measure the thermal stability of the studied substances ( Figure 3a). The decomposition temperature of L-MA is about 145 • C and the decomposition temperature of the H 2 mba ligand of Ag 9 -NCs is about 200 • C. After assembly, the decomposition temperature of the H 2 mba ligand of Ag 9 -NCs for Ag 9 -NCs/L-MA xerogel is about 260 • C, indicating that the stability of Ag 9 -NCs is further improved by supramolecular self-assembly.  Small-angle X-ray spectroscopy (SAXS) and X-ray diffraction (XRD) can effectively characterize the deposition pattern and spatial structure of the xerogels. SAXS shows that Ag9-NCs/L-MA xerogel exhibits four scattering peaks, and the scattering factor q ratio is Fourier transform infrared (FT-IR) is an effective tool for analyzing the supramolecular forces ( Figure 3b). The broad peak of Ag 9 -NCs/L-MA xerogel at 2500 cm −1 to 3200 cm −1 represents the stretching vibration of the hydroxyl group, which is stronger and wider than that of Ag 9 -NCs, indicating the formation of hydrogen bonds in the system. The peak at 1700 cm −1 representing the stretching vibration of the C=O in the carboxyl group becomes weaker than that of L-MA after the gel is formed, and slightly shifts to a lower wave number, which represents the formation of hydrogen bonds and confirms that L-MA participates in the construction of the hydrogel. The peak at 3540 cm −1 represents that the hydroxyl groups in L-MA undergo intermolecular association through hydrogen bonds to form L-MA dimers, which disappear after gelation, indicating that L-MA forms hydrogen bonds with the peripheral ligands of Ag 9 -NCs. The peaks at 1537 cm −1 and 1377 cm −1 belong to the antisymmetric and symmetric stretching vibration of C=O in carboxylate from ligand of Ag 9 -NCs. For Ag 9 -NCs/L-MA xerogel, the peak of C=O in carboxylate moves, which further confirms the formation of hydrogen bonds between ligand of Ag 9 -NCs and L-MA. Moreover, it can be seen that the absorption peak at 900 cm −1 , representing O-H in the carboxyl group of L-MA is strong and after the hydrogel is formed, this peak becomes weaker and narrower, confirming that most of the carboxyl groups of L-MA are involved in the formation of hydrogen bonds, limiting the bending vibration of the O-H bonds in the carboxyl groups.
Small-angle X-ray spectroscopy (SAXS) and X-ray diffraction (XRD) can effectively characterize the deposition pattern and spatial structure of the xerogels. SAXS shows that Ag 9 -NCs/L-MA xerogel exhibits four scattering peaks, and the scattering factor q ratio is 1 : which is a tetragonal stack (Figure 3c). The smallest repeating unit of the aggregate d = 1.36 nm (d = 2π/q), which is equivalent to the size of Ag 9 -NCs. From the XRD results, it can be observed that L-MA is a triclinic crystal system, while the peak of Ag 9 -NCs/L-MA xerogel at 2θ = 20-40 • represents various possible regular arrangements of atomic layers in assembled nanostructures, which is very different from L-MA and Ag 9 -NCs (Figure 3d), indicating Ag 9 -NCs and L-MA formed a multi-complex during the self-assembly. According to the Bragg equation, the interplanar distances of the atomic layer are in the range of 2.37-3.81 Å. Diffraction peaks at 2θ = 30.72 correspond to Ag-Ag, indicating that the d10-d10 argentophilic interaction may exist in the Ag 9 -NCs/L-MA xerogel [40,41,43].
The rheological characteristics are of great significance for supramolecular hydrogels, and the mechanical strength of the Ag 9 -NCs/L-MA hydrogels can be evaluated by the rheological measurement. In the stress scanning (Figure 3e), the storage modulus (G = 16,900 Pa) is much larger than the loss modulus (G" = 614.6 Pa), indicating that the hydrogels exhibit a solid-like nature. The Ag 9 -NCs/L-MA hydrogels exhibit good viscoelasticity, a wider linear viscoelastic region, and a higher yield stress (892.8 Pa), indicating that the hydrogels constructed by the Ag 9 -NCs are more rigid and exhibit strong damage resistance. In the frequency sweep test ( Figure S4), G is larger than G" and the moduli of the hydrogels are almost independent of the applied frequency. The above results indicate that the Ag 9 -NCs/L-MA hydrogels have high mechanical strength.
The circular dichroism (CD) spectrum has further confirmed that the Ag 9 -NCs/L-MA hydrogel possesses supramolecular chirality. L-MA has a positive Cotton effect at 212 nm and no obvious CD signal was detected in the Ag 9 -NCs aqueous solution. But the Ag 9 -NCs/L-MA hydrogel has a positive Cotton effect at 230 nm, and the original CD signal of L-MA disappears. Moreover, we also used D-MA to construct Ag 9 -NCs/D-MA hydrogel and it is interesting to find that the CD spectrum of the Ag 9 -NCs/D-MA hydrogel is exactly opposite of the Ag 9 -NCs/L-MA hydrogel. It can be concluded that through supramolecular self-assembly, the molecular chirality of L-MA (or D-MA), was successfully transferred to the supramolecular level, which induced the Ag 9 -NCs/L-MA hydrogel (Ag 9 -NCs/D-MA hydrogel) has supramolecular chirality (Figure 3f).

Ag 9 -NCs/L-MA Xerogel/PMMA Film for Sensing
The composite material obtained by doping the xerogel into the polymer matrix has the advantages of easy processing and good flexibility and can enhance the practical application of the gel [32,33]. PMMA has good UV resistance, chemical durability, and good mechanical properties. Therefore, based on the excellent sensing performance of metal NCs and the advantages of simple preparation of organic films as a matrix material, Ag 9 -NCs/L-MA xerogel are introduced into the organic glass matrix to form a new type of organic film. Herein, the 8 mM Ag 9 -NCs/0.3 M L-MA xerogel is introduced into the PMMA, and through the solvent volatilization method to get a hybrid film. Firstly, several films were prepared with different doping concentration of 8 mM Ag 9 -NCs/0.3 M L-MA xerogel and it can be observed that as the doping concentration increases (from 0.1% to 0.4%), the fluorescence intensity increases but the transmittance decreases (Figure 4a-c). Integrating transmittance and fluorescence spectra, a composite Ag 9 -NCs/L-MA/PMMA film with a mass concentration of 0.3% xerogel was selected to study its sensing performance.
L-MA disappears. Moreover, we also used D-MA to construct Ag9-NCs/D-MA hydrogel and it is interesting to find that the CD spectrum of the Ag9-NCs/D-MA hydrogel is exactly opposite of the Ag9-NCs/L-MA hydrogel. It can be concluded that through supramolecular self-assembly, the molecular chirality of L-MA (or D-MA), was successfully transferred to the supramolecular level, which induced the Ag9-NCs/L-MA hydrogel (Ag9-NCs/D-MA hydrogel) has supramolecular chirality (Figure 3f).

Ag9-NCs/L-MA Xerogel/PMMA Film for Sensing
The composite material obtained by doping the xerogel into the polymer matrix has the advantages of easy processing and good flexibility and can enhance the practical application of the gel [32,33]. PMMA has good UV resistance, chemical durability, and good mechanical properties. Therefore, based on the excellent sensing performance of metal NCs and the advantages of simple preparation of organic films as a matrix material, Ag9-NCs/L-MA xerogel are introduced into the organic glass matrix to form a new type of organic film. Herein, the 8 mM Ag9-NCs/0.3 M L-MA xerogel is introduced into the PMMA, and through the solvent volatilization method to get a hybrid film. Firstly, several films were prepared with different doping concentration of 8 mM Ag9-NCs/0.3 M L-MA xerogel and it can be observed that as the doping concentration increases (from 0.1% to 0.4%), the fluorescence intensity increases but the transmittance decreases (Figure 4a-c). Integrating transmittance and fluorescence spectra, a composite Ag9-NCs/L-MA/PMMA film with a mass concentration of 0.3% xerogel was selected to study its sensing performance. Then, 0.3% Ag9-NCs/L-MA xerogel/PMMA films were placed into different metal cation aqueous solutions for 10 min and then, the luminescence spectra of these films were studied (Figures S5 and S6). It is obviously that the composite film shows an obvious quenching effect only toward Fe 3+ (Figure 5a,b). Furthermore, the 0.3% Ag9-NCs/L-MA xerogel/PMMA films were placed into aqueous solutions containing different concentrations of Fe 3+ ions for 10 min to study the corresponding luminescence intensity ( Figure  5c,d). With the gradual increase of cFe3+, the luminescence intensities at 628 nm are significantly weakened. In order to investigate the luminescence quenching efficiency, the Stern-Volmer (S-V) equation was used to quantitatively analyze the quenching curve [32]:  Then, 0.3% Ag 9 -NCs/L-MA xerogel/PMMA films were placed into different metal cation aqueous solutions for 10 min and then, the luminescence spectra of these films were studied (Figures S5 and S6). It is obviously that the composite film shows an obvious quenching effect only toward Fe 3+ (Figure 5a,b). Furthermore, the 0.3% Ag 9 -NCs/L-MA xerogel/PMMA films were placed into aqueous solutions containing different concentrations of Fe 3+ ions for 10 min to study the corresponding luminescence intensity (Figure 5c,d).
With the gradual increase of c Fe3+ , the luminescence intensities at 628 nm are significantly weakened. In order to investigate the luminescence quenching efficiency, the Stern-Volmer (S-V) equation was used to quantitatively analyze the quenching curve [32]: where I 0 and I are the luminescence intensity at 640 nm when c = 0 and c = M, respectively, K SV is the quenching coefficient of Fe 3+ ions, and [M] is the molar concentration of Fe 3+ ions. The quenching curve shows a well-fitted linear relationship at low c Fe3+ (1-100 µM).
The K SV value was calculated to be 2.3 × 10 4 M −1 . According to the detection limit expression defined by IUPAC, the detection limit of the composite membrane is calculated to be 0.3 µM, which indicates that the as-prepared 0.3% Ag 9 -NCs/L-MA xerogel/PMMA film material exhibited good sensing performance. The limit of detection of the Ag 9 -NCs/L-MA xerogel/PMMA film far less than the maximum concentration of Fe(III) in drinking water of 5.36 µM (specified by the Minister of Health of the People's Republic of China). KSV value was calculated to be 2.3 × 10 4 M −1 . According to the detection limit expression defined by IUPAC, the detection limit of the composite membrane is calculated to be 0.3 μM, which indicates that the as-prepared 0.3% Ag9-NCs/L-MA xerogel/PMMA film material exhibited good sensing performance. The limit of detection of the Ag9-NCs/L-MA xerogel/PMMA film far less than the maximum concentration of Fe(III) in drinking water of 5.36 μM (specified by the Minister of Health of the People's Republic of China).  (Figure 5e,f), it can be seen that the fluorescence is still quenched in the presence of other competing metal cations, which indicates that the composite film has satisfactory selectivity for Fe 3+ detection. In addition, the used films were picked out and washed with distilled water several times, and the corresponding luminescence intensities cannot be recovered. Therefore, it would be used as a disposable test strip for detection Fe 3+ ions in drinking water in the future.
The possible sensing mechanism of Fe 3+ ions quenching the fluorescence of 0.3% Ag9-NCs/L-MA xerogel/PMMA film was further analyzed. It can be seen from UV-Vis ( Figure  6a) that the absorption peaks of Fe 3+ and the Ag9-NCs/L-MA hydrogel overlap in the absorption range, indicating that the competitive absorption of Fe 3+ reduces the energy transfer efficiency [42]. Moreover, structural collapse or change maybe also cause the luminescence to be quenched [32]. The XRD test was performed on the Ag9-NCs/L-MA xerogel before and after immersion in Fe 3+ ion aqueous solution (Figure 6b) (Figure 5e,f), it can be seen that the fluorescence is still quenched in the presence of other competing metal cations, which indicates that the composite film has satisfactory selectivity for Fe 3+ detection. In addition, the used films were picked out and washed with distilled water several times, and the corresponding luminescence intensities cannot be recovered. Therefore, it would be used as a disposable test strip for detection Fe 3+ ions in drinking water in the future.
The possible sensing mechanism of Fe 3+ ions quenching the fluorescence of 0.3% Ag 9 -NCs/L-MA xerogel/PMMA film was further analyzed. It can be seen from UV-Vis (Figure 6a) that the absorption peaks of Fe 3+ and the Ag 9 -NCs/L-MA hydrogel overlap in the absorption range, indicating that the competitive absorption of Fe 3+ reduces the energy transfer efficiency [42]. Moreover, structural collapse or change maybe also cause the luminescence to be quenched [32]. The XRD test was performed on the Ag 9 -NCs/L-MA xerogel before and after immersion in Fe 3+ ion aqueous solution (Figure 6b). The XRD spectra of the samples were not consistent, which means that the structure of the Ag 9 -NCs/L-MA xerogel was destroyed after treated by Fe 3+ ion aqueous solution. Therefore, the collapse of the crystal structure is also one of the reasons for the quenching of luminescence. Thus, it can be concluded that the fluorescence quenching of Ag 9 -NCs/L-MA xerogel/PMMA film is caused by the competitive absorption of Fe 3+ and the destruction of the crystal structure. The fluorescence quenching phenomenon of the Ag 9 -NCs/L-MA xerogel/PMMA film is shown in Scheme 1. xerogel was destroyed after treated by Fe 3+ ion aqueous solution. Therefore, the collapse of the crystal structure is also one of the reasons for the quenching of luminescence. Thus, it can be concluded that the fluorescence quenching of Ag9-NCs/L-MA xerogel/PMMA film is caused by the competitive absorption of Fe 3+ and the destruction of the crystal structure. The fluorescence quenching phenomenon of the Ag9-NCs/L-MA xerogel/PMMA film is shown in Scheme 1.

Conclusions
In summary, through self-assembly, Ag9-NCs, and L-MA formed a supramolecular hydrogel, with highly ordered aggregates, by regulating a variety of non-covalent interactions. The nanostructure (tangled hollow tubes) in the hydrogel indicated that L-MA restricts the intramolecular vibration and rotation of the ligand of the Ag9-NCs, so that it can emit a stable and bright orange-red phosphorescent emission. The excellent photoluminescence properties of Ag9-NCs/L-MA xerogel make it likely to be used as highly sensitive probes for Fe 3+ . The Ag9-NCs/L-MA xerogel/PMMA composite film can selectively identify Fe 3+ , the quenching coefficient KSV is 2.3 × 10 4 M −1 , and the detection limit is 0.3 μM. The composite film also possesses good recyclability and anti-interference ability, with respect to another ions. The current research aims to achieve AIE, by precisely regulating the formation of ordered aggregates of metal NCs, broadening the research field of metal NCs, and enriching the practical applications of these luminescent materials.

Materials
Ag9-NCs was synthesized and purified, according to our previous work, which have a crystal structure [44]. L-MA and D-MA were purchased from Sinopharm Chemical Reagent Co (Shanghai, China) and used without further purification. Ultrapure water used in the experiments, with a resistivity of 18.25 MΩ cm −1 , was obtained using a UPH-IV ultrapure water purifier (Sichuan, China). Polymethylmethacrylate (PMMA, average Mw: ~350,000) was purchased from Sigma-Aldrich (Shanghai, China). Dichloromethane (CH2Cl2) were obtained from local supplier with the quality of analytical grade and used without further purification.

Conclusions
In summary, through self-assembly, Ag 9 -NCs, and L-MA formed a supramolecular hydrogel, with highly ordered aggregates, by regulating a variety of non-covalent interactions. The nanostructure (tangled hollow tubes) in the hydrogel indicated that L-MA restricts the intramolecular vibration and rotation of the ligand of the Ag 9 -NCs, so that it can emit a stable and bright orange-red phosphorescent emission. The excellent photoluminescence properties of Ag 9 -NCs/L-MA xerogel make it likely to be used as highly sensitive probes for Fe 3+ . The Ag 9 -NCs/L-MA xerogel/PMMA composite film can selectively identify Fe 3+ , the quenching coefficient K SV is 2.3 × 10 4 M −1 , and the detection limit is 0.3 µM. The composite film also possesses good recyclability and anti-interference ability, with respect to another ions. The current research aims to achieve AIE, by precisely regulating the formation of ordered aggregates of metal NCs, broadening the research field of metal NCs, and enriching the practical applications of these luminescent materials.

Materials
Ag 9 -NCs was synthesized and purified, according to our previous work, which have a crystal structure [44]. L-MA and D-MA were purchased from Sinopharm Chemical Reagent Co (Shanghai, China) and used without further purification. Ultrapure water used in the experiments, with a resistivity of 18.25 MΩ cm −1 , was obtained using a UPH-IV ultrapure water purifier (Sichuan, China). Polymethylmethacrylate (PMMA, average Mw:~350,000) was purchased from Sigma-Aldrich (Shanghai, China). Dichloromethane (CH 2 Cl 2 ) were obtained from local supplier with the quality of analytical grade and used without further purification.

Synthesis of Ag 9 -NCs/L-MA Hybrid Nanostructures
In this experiment, 0.5 mL of Ag 9 -NCs solution (15.87 mM) was added to 0.5 mL L-MA solution (0.6 M) with stirring. The hydrogel was successfully prepared after 8 h of constant temperature (20 • C) in a thermostat. The hydrogels was lyophilized in a vacuum extractor at 60 • C for 5 day to collect the orange-yellow powder.

Fabrication of Ag 9 -NCs/L-MA/PMMA Composite Thin Film
The PMMA powder (200 mg) was dissolved in dichloromethane (8 mL), then followed by addition of the corresponding required of orange-yellow Ag 9 -NCs/L-MA xerogels. After being evenly dispersed, place it in a petri dish with a diameter of 6 cm at room temperature for 5 h. Each set of data has been measured 3 times using different batches of film to reduce the error.

Characterization
A copper mesh was inserted into the gel to obtain a sample and, after drying under an IR lamp for 45 min, TEM images were observed under a JCR-100CX II (JEOL) microscope. The gel was placed on a silica wafer, dried for 45 min under an IR lamp, and observed by field-emission SEM and AFM, respectively. UV−vis data were recorded on a Shimadzu UV-2600 spectrophotometer. Fluorescence data were tested on an LS-55 spectrofluorometer (PerkinElmer, Waltham, MA, USA) and an Edinburgh Instruments FLS920 luminescence spectrometer (xenon lamp, 450 W), respectively. SAXS measurements were performed using an Anton-Paar SAX Sess mc 2 system with nickel-filtered Cu Kα radiation (1.54 Å) operating at 50 kV and 40 mA. XRD patterns were taken on a D8 ADVANCE (Germany Bruker) diffractometer, equipped with Cu Kα radiation and a graphite monochromator. FT-IR spectra in KBr wafer were recorded on a VERTEX-70/70v spectrophotometer. CLSM observations were performed using an inverted microscope (model IX81, Olympus, Tokyo, Japan), equipped with a high-numerical-aperture 60 oil-immersed objective lens. The rheological measurements were carried out on an Anton-Paar Physica MCR302 rheometer with a cone-plate system. Before the frequency sweep, an amplitude sweep at a fixed frequency of 1 Hz was carried out to ensure that the selected stress was in the linear viscoelastic region. The frequency sweep was carried out from 0.01 to 100 Hz at a fixed stress of 10 Pa. TGA was performed under a nitrogen atmosphere at 25-700 • C, with a heating speed of 10 • C min −1 on a TA SDT Q600 thermal analyzer. CD spectra were obtained using a JASCO J-810 spectropolarimeter, which was flushed with nitrogen during operation. The absolute fluorescence quantum yields were measured with a spectrofluorometer (FLSP920, Edinburgh Instruments Ltd., Livingston, UK), equipped with an integrating sphere.
Supplementary Materials: The following are available online at https://www.mdpi.com/article/ 10.3390/gels7040192/s1, Figure S1: The molecular structure of Ag 9 -NCs, Figure S2: AFM image of fibers, Figure S3: (a-b) TEM image of the fibers. (c-d) SEM image of fibers, Figure S4: Elastic modulus (G ) and viscous modulus (G") as a function of the applied stress at a constant frequency (1.0 Hz), Figure S5: Photographs of Ag 9 -NCs/L-MA xerogel/PMMA film under different conditions, Figure S6: Luminescence emission spectra of 0.3% Ag 9 -NCs/L-MA xerogel/PMMA film in 100 µM Fe 3+ aqueous solution with different interaction time, Table S1: The average lifetime of Ag 9 -NCs and hydrogel.
Funding: This research received no external funding.